Stress-induced stabilization of pyrolyzed polyacrylonitrile and carbon
nanotubes electrospun fibers
Paola Serena Ginestra1&Elisabetta Ceretti1 Received: 27 June 2019 / Accepted: 17 April 2020
# Springer-Verlag London Ltd., part of Springer Nature 2020
The unique properties of graphitic carbons have gained widespread attention towards their development and application. Carbon materials can be synthesized by thermal decomposition and, more specifically, carbon pyrolysis from polymer precursors. The paper shows the pyrolysis process of polyacrylonitrile (PAN) in the presence of multi-walled carbon nanotubes (MWCNTs) according to different manufacturing process conditions. The electrospinning process of the PAN-MWCNTs solution on multi-plates collectors was firstly analyzed. The morphology and the particles arrangement of the electrospun fibers was studied under scanning and transmission electron microscopes. Moreover, the composite fibrous mats were characterized by RAMAN spec-troscopy to identify the effects of a mechanical tension application during the thermal stabilization phase performed before the pyrolysis treatment to obtain carbon fibers from the precursor polymer. The results show that the graphitization of the pyrolyzed fibers is enhanced by the combination of MWCNTs and a mechanical stress applied during the thermal treatment.
Keywords Electrospinning . Carbon . Nanomanufacturing . Pyrolysis
Polymer fibers are used for diverse applications. According to the last estimates, the world consumption of fibers is reaching 60 million tons per annum [1,2]. Polymer nanofiber networks are being considered as filters, scaffolds for tissue engineer-ing, protective clothengineer-ing, reinforcements in composite mate-rials, and sensors [3–5]. Although some of these applications are in the development stage, a few have been commercially exploited . Carbon-based materials have gained interest for the attractive electronic and structural properties and the in-trinsic electrochemical stability useful for a variety of techno-logical applications. A carbon fiber (CF) is defined as a fiber containing at least 92 wt% of carbon, while a fiber containing at least 99 wt% carbon is usually called a graphite fiber . Almost all CFs are produced from pyrolysis of precursor fi-bers. The current carbon fiber market is dominated by poly-acrylonitrile (PAN) carbon fibers, while the rest is related to pitch carbon fibers and a very small amount of rayon carbon
fiber textiles [8,9]. The optimization of the pyrolysis process of the PAN precursor fibers would ideally result in enhanced performances of the resulting CF [10,11]. Pyrolytic carbon fibers are chemically stable and exhibit a wide potential win-dow but require post-processing to be effective especially in sensing applications. Nanoparticles can change the structural and physical properties of the fibers as reinforcement agents. The most used nanoparticles to reinforce nanofibers are car-bon nanomaterials and especially nanotubes and graphene . The growing expansion of new carbon materials resulted in an expansion of the theoretical research on the correlation between the microstructural changes induced by these nano-particles and the synthesis of carbon-enriched materials [13,
14]. Carbon nanotubes (CNTs) and graphene nanosheets have been studied in the last two decades and a lot of research has been focused on these two carbon allotropes combined with polymer nanocomposites . However, the production of carbon-based materials with tailorable properties has still to be fully understood despite their continuous industrial use. On the other hand, the production of carbon substrates, such as electrodes, is challenging due to the expensive costs of the fabrication. Moreover, the relationship between the synthesis and structure of new carbon materials is still uncertain despite their widespread use in industry. Anyhow, CFs possessing high degree of preferred orientation of the graphene layers
* Paola Serena Ginestra email@example.com
1 Department of Mechanical and Industrial Engineering, University of
Brescia, V. Branze 38, 25123 Brescia, Italy
are known to exhibit optimal properties in terms of electrical and thermal conductivity and promising mechanical properties.
Here, the authors demonstrate how the effects of a mechan-ical treatment can significantly enhance the precursor fibers graphitization by the specific rearrangement of the organic material in relation to CNTs. The aim of the study was to understand whether PAN fibers may be graphitized at a lower pyrolysis temperature compared to the commercially available PAN-based CFs , challenging the present approaches concerning the graphitization of polymers. Carbon composites have extensively been developed using PAN fibers heat-treated to temperatures between 1000 and 2500 °C . The overall structure of PAN-based carbon fibers remains that of a hard carbon, thus non-graphitic, till 2000 °C, and the transfor-mation of the structure into a graphitic carbon, usually derived from soft carbon, is achieved above 2500 °C. The reduction of the temperature required to obtain graphitic carbon from a polymer precursor is therefore crucial to spread the application of this technique. The graphitization of organic precursor has been attributed to their chemical and physical properties that can prevent the formation of graphitic planes without a rear-rangement of the carbon atoms in the fusion phase occurring during the heat treatment. Subsequently, alternative strategies are being investigated to induce graphitization in polymer precursors . In this work, the electrospinning process of PAN enriched with multi-walled CNTs was used to enhance the orientation of the precursor’s chains that was preserved with the application of a mechanical stress during the thermal stabilization prior to pyrolysis. The extent of graphitization of PAN-CNTs fibers is found to be dependent on the fibers-nanoparticles interactions . Previous works already fo-cused on the characterization of PAN-CNTs electrospun fi-bers. The glass transition temperature (Tg) of PAN fibers can be modified by 3 °C with the insertion of CNTs due to the reduction of mobility of the PAN chains [20,21]. In particular, an increase of the Tg of PAN-CNTs fibers has been observed by incorporating 0.75 wt% of CNTs into the PAN matrix but the Tg increasing trend is reduced at higher CNTs contents due to a progressive lower interaction between the nanoparti-cles and the polymer chains. Moreover, the chemical compo-sition, before and after carbonization, of PAN-CNTs fibers has been deeply investigated  showing that the addiction of CNTs contributes to orient the crystallization of the PAN mo-lecular chains during the spinning process leading to a higher crystal perfection of the PAN polymer in the PAN-CNTs com-posite. These results highlighted the potential role of the CTNs as a template to maintain the polymer extended chain config-uration during carbonization .
The nanoparticles arrangement was evaluated under EDS, TEM (HRTEM; FEI, Titan 80–300 kV S/TEM), and RAMAN spectroscopy (Renishaw InVia Raman Microscope), while the effects of the mechanical tension during thermal stabilization
prior to the pyrolysis treatment were analyzed and characterized by RAMAN spectroscopy and SEM (Hitachi Regulus 8230 ultra-high resolution SEM).
2 Electrospinning and pyrolysis
The first step for the production of the electrospinning solution is the suspension of 1% MWCNTs (diameter of 110–170 nm, length 5–9 μm) in dimethylformamide (DMF) followed by sonication for 1 h at 35 °C. Three homogeneous solutions of 8 wt% of PAN (150,000 g/mol) were prepared by adding the polymer to the MWCNTs solution as previously reported [24,
25]. The MWCNTs-PAN solution was then stirred for 48 h at 30 °C. The electrospinning tests were carried out with the newly formulated solutions and the collected fibers were char-acterized to analyze the interaction between the nanotubes and the polymer. The electrospinning was carried out by applying a flow rate of 0.8 ml/h to a 10-ml syringe equipped with a 21 Gauge needle. The voltage applied between the needle and the collector was 12 kV and the distance between the needle tip and the collector was kept at 210 mm. Furthermore, two dif-ferent copper collectors were used: one single square collector and a multi-plates collector. The geometry of the collector can have a strong influence on the deposition of the fibers accord-ing to the direction of the electrical field. In this context, a multi-plates collector allows the alignment the fibers along one parallel direction by the generation of an ordered electric field towards the plates [26,27]. On the other hand, the fibers are randomly deposited on the square collector due to the uniformity of the electrical field on the grounded collector. The process was run for 30 min and the tests were performed at ambient conditions of 25 °C and relative humidity of 40% . The obtained fibers were then thermally stabilized prior to the carbonization (Fig.1). Since the heating rate determines the evolution rate of volatile components from PAN fibers and consequently affects the performance of the carbon fibers, a temperature of 280 °C was applied for 6 h. The samples sta-bilized are then submitted to carbonization in a nitrogen envi-ronment at an approximate flow rate of 4600 sccm in order to remove all the non-carbon elements and obtain fibers made by pristine carbon . The temperature and the time of exposure in this step are as fundamental as for the stabilization.
The temperature, starting from 20 °C (room temper-ature), is increased for 60 min until it reaches 300 °C, so the ramp is 4 °C/min. Then, the temperature is main-tained for 60 min at 300 °C to complete the preliminary stage of the process of the pre-carbonization. At this point, the temperature is increased again until the tem-perature achieves 1050 °C: the ramp in this case is 2.5 °C/min . During this step, the second and the final stages of the process of the pre-carbonization are carried out.
When the temperature reaches 1050 °C, the process of carbonization takes place and the temperature is kept constant for 60 min in order to finish the process. All the analyses presented in the following sections have been carried out on pyrolyzed samples.
2.1 MWCTNs-PAN fibers
The elemental composition of the MWCNTs-PAN samples obtained on the square collector was analyzed with SEM-EDS mapping as shown in Fig.2.
The quantitative elemental composition of the MWCNTs-PAN fibers before (Fig.2a) and after (Fig.2b) pyrolysis re-veals the presence of oxygen due to the chemical reactions occurring during the stabilization of PAN as a carbon fiber precursor . The variation of the nitrogen content can be attributed to the polyacrylonitrile composition (C3H3N)nthat is carbonized by pyrolysis carried out in a controlled nitrogen atmosphere.
The distribution and arrangement of the MWCNTs was analyzed under TEM operating at 300 kV. Figure3ashows
that MWCNTs-PAN samples have no porosity or other de-fects, except for a small surface roughness. The examination of the lattice fringes in the micrographs shows the effects of the carbon microstructures on the fibers developed by the electrospinning process. The MWCNTs-PAN selected area of the diffraction pattern, taken from a thin area of the fibers network, shows concentered circles that are formed from mul-tiple sets of six-fold-symmetrical spots (Fig.3b). This pattern is due to multi-layers of sp2 hybridized carbon planes (from MWCNTs and/or grown carbon crystals) with random orien-tation with respect to the incident electron beam. MWCNTs-PAN fibers present a multi-layer wall of the carbon nanotube and some initial ordering in the shell region near the surface of the nanofiber. This can be better noticed from Fig.3cin which a detail of the fiber’s microstructure is shown.
Close to the surface (a), it is possible to distinguish the orientation of the fringes that indicates a good alignment of the MWCNTs along the fiber axis, while in the core (b), the crystals are randomly oriented. This demonstrates the well-known distinction between the core and shell regions on PAN-precursor nanofibers. The distance between the fringes
Fig. 2 EDS spectrum and chemical composition of MWCNTs-PAN fibers before (a) and after (b) pyrolysis
Fig. 1 Schematic illustration of the micro fabrication process of the pyrolyzed electrospun fibers
indicates the distance between the different layers. The aver-age crystallite thicknessLcresulted in 15.1 ± 4.9 nm.
In particular, PAN is a non-graphitized polymer and the structure of the pyrolyzed PAN is indeed disordered and randomly curled . In this case, the MWCNTs-PAN samples exhibit aligned carbon fringes stacked together and generally well-oriented especially on the shell region of the fibers while the graphene planes become imperfect in the core region of the electrospun fibers. With the addi-tion of CNTs, the nanostructure of pyrolyzed PAN fibers appears more graphitic.
RAMAN spectroscopy allows the quantification of the de-gree and the uniformity of graphitization of the material. The positions, shapes, and intensities of the RAMAN peaks can provide fundamental information about the structural charac-teristics of the carbon fibers. Three spectra were acquired and averaged across each replica to evaluate the graphitic quality of the resulting carbons. The typical RAMAN spectrum (λexcitation= 532 nm) collected across the electrospun MWCNTs-PAN carbon fibers is shown in Fig.4.
The G peak, centered on 1560–1610 cm−1, is related to the in-plane vibrations of pairs of sp2hybridized carbon atoms. The reason for this is that graphite is composed of sp2-bonded carbon in planar sheets in which the bond energy of the sp2 bonds pushes the vibrational frequency of the bonds and hence the frequency of the band in the Raman spectrum. As a result, the intensity and sharpness of the G peaks are signi-fying the presence of crystalline graphitic phase in the synthe-sized material. The D peak at 1300–1400 cm−1is related to the deviation from a perfect graphitic microstructure and thus in-dicates the level of disorder in graphitic sp2structures. The
nature of this peak is related to one-phonon elastic scattering and it is interpreted as a measure of the quantity of sp3or dangling sp2bonds that are causing structural disorders. In this case, the prominent D band in relation to the G band can be attributed to the MWCNTs, given the multi-layer con-figuration, and indicates a certain degree of disorder in the structure.
The quality of graphitization can be evaluated by the D/G peaks ratio. In particular, a low D/G ratio corresponds to a high level of graphitization within the carbon. Moreover, a uniform RAMAN mapping of the carbon fibers is related to an enhanced graphitization throughout the nanofibrous mats. From Fig.4, it is possible to see that MWCNTs-PAN samples present a G-peak higher than the D-peak and it can be seen that in certain points, the value of D/G ratio is around 0.5: this means that the presence of MWCNTs helps the graphitization, raising the intensity of G-peak, and the order of the carbon phase, lowering the D-peak. On the other hand, the typical G′ peak (> 2600 cm−1) is not visible in the graph, reasonably due to the overlapped multilayers of disordered graphene and pos-sible oxygenated functional groups. In fact, the G′ peak cor-responds to a two-phonon band allowed in the second-order Raman spectra of graphene without any kind of disorder or defects .
2.2 Single square vs multiple plates collector
The samples MWCNTs-PAN-SQ and MWCNTs-PAN-MP differs according to the collector used during the electrospinning for each sample: MWCNTs-PAN-SQ is
Fig. 3 Bright field images of the MWCNTs-PAN samples (a, b). Detail of the microstructure of the MWCNTs-PAN nanofiber (c)
obtained with the square collector; MWCNTs-PAN-MP is ob-tained with the multi-plates collector (Fig.5).
Hence, the sample MWCNTs-PAN-SQ shows randomly oriented fibers (Fig.6a) and the sample MWCNTs-PAN-MP shows fibers oriented in a preferential direction (Fig.6b). The direction of the alignment corresponds to the normal direction to the axes of the plates.
3 Stress induction during thermal
The precursor carbon fibers are thermally stabilized un-der ambient air pressure to acquire infusible and nonburning characteristics prior to the carbonization stage. During the thermal stabilization stage, the PAN-CNTs fibers are characterized by a reduction in fiber diameter together with color changes from white to
reddish brown . Since the application of mechanical tension during the thermal stabilization is crucial in order to prevent the polymer chains from relaxing and losing their orientation, two ways of mechanical stretching of samples were designed for each sample. Firstly, a com-pression stress has been applied to the mats and then a tensile stress was chosen to evaluate the effects of this stress on aligned fibers. To allow the application of a c o m p r e s s i o n s t r e s s , t h e M W C N Ts - PA N - S Q a n d MWCNTs-PAN-MP fibrous mats were detached from the collectors and placed between two washers main-tained by two clamps to obtain a compression of 15% (Fig. 7a). On the other hand, the MWCNTs-PAN-MP fibrous mats were also subjected to a uniaxial tensile stress applied by a vise to obtain an elongation of 20% in the longitudinal direction (Fig. 7b).
A summary of the experimental tests and applied condi-tions is reported in Table1.
Fig. 4 RAMAN spectrum and D/G ratio mapping of MWCNTs-PAN fibers
Fig. 5 Square (a) and multi-plates (b) collectors. The insets of the lower corners show the optical microscope images of the as electrospun MWCNTs-PAN fibers on the square and multi-plates collectors
3.1 Compression stress application effects: single
Three samples of MWCNTs-PAN-SQ fibers randomly orient-ed on the square collector were subjectorient-ed to a compressive stress during the thermal stabilization prior to pyrolysis and then pyrolyzed. The comparison between unstressed MWCNTs-PAN-SQ and stressed MWCNTs-PAN-SQ-CS fi-bers is reported in Fig.8(SEM) and Fig.9(RAMAN).
As shown in Fig.8, the compression does not affect the orientation of the fibers. It is possible to conclude that the applied load is not causing a re-orientation of the fiber.
Thus, the fundamental supramolecular structure of the PAN nanofibers is established during the electrospinning process.
Figure9presents the RAMAN shifts for a specific point of the samples MWCNTs-PAN-SQ and MWCNTs-PAN-SQ-CS.
In both the spectra, the D-peak and the G-peak are present. The G-peak is higher than the D-peak in both the samples due to the presence of MWCNTs in the mat, but in the MWCNTs-PAN-SQ-CS sample, the D-peak is lower than the D-peak of the sample MWCNTs-PAN-SQ. This may depend on the me-chanical treatment at which sample MWCNTs-PAN-SQ-CS is subjected during stabilization: the applied stress prevents the polymer chains from relaxing and losing their orientation. That means that the microstructure is more ordered: the D-peak lowers and the G′ D-peak is clearly visible on the spectrum. The reduction of the intensity of the disorder-associated peak reveals a possible increase in the graphitic structure of the mechanically treated samples. Moreover, broader RAMAN peaks are related with a higher level of disorder and defects in the graphitic material. In this case, it is possible to remark a reduction of the areas of both G and D peaks.
Figure10shows that the average value of the D/G ratio of sample MWCNTs-PAN-SQ ( 0.5) is lower than the one of sample MWCNTs-PAN-SQ-CS, but the punctual value of D/G ratio reaches lower values in sample MWCNTs-PAN-SQ-CS. This effect can be attributed to the application of a mechanical tension during stabilization that can enhance the microstructural order of the fibers. The average D/G ratio for sample MWCNTs-PAN-SQ-CS is around 0.8 (ranging from 0.6 to 1). This value can be attributed to an incomplete disper-sion of the MWCNTs in the polymer solution.
Fig. 6 SEM images of MWCNTs-PAN-SQ (a) and MWCNTs-PAN-MP (b) fibers. The average diameter of the fibers is 132.2 ± 15 nm (porosity = 5.03%) for the MWCNTs-PAN-SQ sample and 169.2 ± 40 nm (porosity = 21%) for MWCNTs-PAN-MP sample
Fig. 7 Washers for the application of the compression stress (a) and vise for the application of the uniaxial tensile stress (b)
Table 1 Summary of the electrospun mats subjected to stress-induced thermal stabilization
Test name Collector Applied stress MWCNTs-PAN-SQ-CS Square Compression MWCNTs-PAN-MP-CS Multi-plates Compression
3.2 Compression stress application effects: multiple
Three samples of MWCNTs-PAN-MP fibers deposited on the multi-plates collector were subjected to the compressive stress during the thermal stabilization prior to pyrolysis and then pyrolyzed. As shown in Fig.9, the compression seems en-hancing the orientation of the MWCNTs-PAN-MP-CS fibers accordingly to their direction given by the multi-plates collec-tor (Fig.11).
It can be concluded that the application of a compression stress is more effective on the already oriented fibers collected on the multi-plates configuration.
The RAMAN spectrum in Fig.12shows similar D and G peak intensities compared to the spectrum in Fig.9b indicat-ing that the compressive stress is not influencindicat-ing the degree of graphitization of the fibers in relation to their orientation.
Considering the mapping of sample MWCNTs-PAN-MP-CS, reported in Fig.12, the average value of D/G ratio results to 0.6 ranging from 0.2 to 0.8. As the stress is uniform on the mat, it is possible to consider the D peak constant and thus that the lowest values of D/G ratio are found in correspondence to the MWCNTs that raise the G-peak.
The average value of the D/G ratio is lower in the MWCNTs-PAN-MP-CS sample if compared to the one relat-ed to the MWCNTs-PAN-SQ-CS sample. This local rrelat-eduction of the D/G ratio can be attributed to the enhanced alignment of the fibers that gives more orientation to the microstructure of the MWCNTs-PAN composite helping the increase of the graphitization degree.
3.3 Compression vs tensile stress: multiple plates
Considering the results of the application of the compression stress on the aligned fibers, a controlled vise was used to subject the MWCNTs-PAN-MP fibrous mats to an elongation ofƐ = 20%.
Figure 13 shows that the sample MWCNTs-PAN-MP-E presents a similar orientation of the fibers compared to the MWCNTs-PAN-MP-CS sample but in this case, it can be seen that the stretching in sample MWCNTs-PAN-MP-E induces more tension on the fibers. The applied tension causes more stress along the fibers’ axes resulting in shorter fibers and randomly distributed cracks. Figure13creports the transition
Fig. 9 Comparison between RAMAN spectra of MWCNTs-PAN-SQ (a) and MWCNTs-PAN-SQ-CS (b) fibers
Fig. 8 Comparison between SEM images of MWCNTs-PAN-SQ (a) and MWCNTs-PAN-SQ-CS (b) fibers. The average diameter of the fibers is 132.2 ± 15 nm (porosity = 5.03%) for the MWCNTs-PAN-SQ sample and 168 ± 30 nm (porosity = 4.38%) for MWCNTs-PAN-SQ-CS sample
of the MWCNTs-PAN fibers from an amorphous nanostruc-ture to a graphitic material with directionally aligned carbon fringes visible on both the shell and core regions of the fiber. In particular, the mechanical tension induced the ordering of the tortuous and randomly oriented carbon planes that became parallel and well-aligned.
In this case, the RAMAN spectrum appears different com-pared to all the previous conditions. The G-peak intensity,
which is affected from the presence of MWCNTs, has the same value of the sample MWCNTs-PAN-MP-CS because the percentage of MWCNTs is the same in both the samples. On the other hand, the G peak area is markedly reduced and
Fig. 12 RAMAN spectrum and D/G ratio mapping of MWCNTs-PAN-MP-CS
Fig. 10 Comparison between the D/G ratio mapping of SQ (a) and MWCNTs-PAN-SQ-CS (b) fibers
Fig. 11 Lower (a) and higher (b) magnification SEM images of MWCNTs-PAN-MP-CS fibers. The average diameter of the fibers is 159 ± 39 nm (porosity = 19.8%)
the D-peak is abruptly lowered due to the tensile tension ap-plied during stabilization that seems to help lower the micro-structural disorder. The sharpness of the G peak is indicating that the bonds are more uniform due to the formation of rela-tively larger nanocrystallines with the mechanical treatment. Both the evolution of the areas of the G and D peaks and the lowered intensity of the D peak are indicating a substantial reduction of the level of disorder and an increase of the graph-itization degree. Moreover, the G′ peak intensity is still lower than the G peak intensity, but the G′ peak increase is probably
attributed to the higher stacking order of the graphene layers. The G′ peak shift in graphite (2700 cm−1) is a result of inter-actions between the stacked graphene layers which result in a tendency to shift the bands to higher frequency (Fig.14).
The average D/G ratio value for the MWCNTs-PAN-MP-E sample is 0.4 ranging from 0.1 to 0.7. The difference between the ratios observed for the MWCNTs-PAN-MP-CS sample leads on the high difference between the D peak values that in this case is lower due to the application of a different stress state.
From these results, it is possible to conclude that the typical crosslinking phase of precursors occurring when heated to 300 °C is partially followed by a fusion phase in which the molecular structure is not totally fixed and the carbon atoms can rearrange themselves allowing the formation of graphitic planes that are more thermodynamically stable . The re-sults highlighted that the use of CNTs is not modifying the graphitization of the carbon fibers obtained by the pyrolysis of the PAN. On the other hand, the graphitization degree can be
Fig. 13 Lower (a) and higher (b) magnification SEM images of MWCNTs-PAN fibers. The average diameter of the fibers is 183 ± 32 nm (porosity = 16.9%). Bright field images of the MWCNTs-PAN-MP-E samples (c)
Fig. 14 RAMAN spectrum and D/G ratio mapping of MWCNTs-PAN-MP-E
enhanced by the implementation of a mechanical treatment in the direction of the alignment of the electrospun fibers that causes the reduction of the relative intensity of disorder of the graphitic material.
4 Conclusion and future trends
This paper reports the characterization of carbon fibers de-rived from the pyrolysis of PAN precursor electrospun fibers. A certain percentage of MWCNTs was added to the polymer solution to study the effects of the presence of nanoparticles on the final orientation and graphitization of the pyrolyzed fibers. The aim was to understand whether PAN fibers may be graphitized at lower pyrolysis temperature compared to the current commercial processes followed for graphitizing poly-mers .
The results show that a multi-plates configuration of the collector can lead to a preferential direction of the fibers but has no effects on the degree of graphitization of the fibers. The MWCNTs-PAN-aligned fibers were subjected to a compres-sion load equally distributed on the fibrous mats to try to preserve the polymer chain alignment. In this case, the D/G ratio mapping showed an interesting difference compared to the previous results, indicating a lower degree of disorder of the carbon phase within the fibers. A tensile stress was then applied to the MWCNTs-PAN aligned fibers and the SEM images showed that the stressed fibers maintained their orien-tation despite of an over tension state effect occurred due to the stretching. In this final case, the RAMAN spectrum and D/G ratio mapping showed remarkable differences compared to the previous results. It can be concluded that, in this case, a lower disorder degree of the carbon phase of the pyrolyzed MWCNTs-PAN fibers, and subsequently, a higher degree of graphitization, was achieved. These results on the pyrolyzed fibers properties indicate that it is possible to tailor the carbon fibers microstructure according to the specific requirements. In particular, this analysis demonstrates that the graphitization of PAN-derived carbon fibers can be correlated to the condi-tions imposed during the stabilization of the precursor poly-mer. The combination of electrospinning, addition of carbon nanotubes and mechanical tension applied has been demon-strated to promote the molecular rearrangement during the heat treatment of PAN precursor enhancing its graphitization at reduced pyrolysis temperature. In particular, the MWCNTs added to the PAN solution influence the dielectrophoretic forces during the electrospinning process producing an align-ment of the polymer molecular chains. Although the graphiti-zation of organic precursors is a complex mechanism that still needs to be fully understood, this work demonstrates that the treatments applied can have a strong influence on the micro-structures of a polymer turned into graphitic carbon providing a promising route to explore new applications of the
graphitization of PAN electrospun fibers. Accordingly, the future research will be focused on the study of the electro-chemical performances of electrospun structures made of py-rolyzed MWCNTs-PAN fibers for sensing and tissue engi-neering applications. In particular, the response of the treated PAN-MWCNTs seems to be increased both as hydrogen per-oxide and iodine sensors as well as when applied for electro-chemical sensing platforms without requiring additional post-processing to functionalize the carbon electrodes .
Acknowledgments The authors would like to acknowledge the support and the assistance of Prof. Marc Madou, Dr. Sunny Holmberg, Dr. Arnoldo Salazar at University of California Irvine and the technical as-sistance of Dr. Michele Norbis.
1. Ginestra P, Ceretti E, Fiorentino A (2016) Electrospinning of poly-caprolactone for scaffold manufacturing: experimental investiga-tion on the process parameters influence. Procedia CIRP 49:8–13 2. Ginestra P, Fiorentino A, Ceretti E (2017) Micro-structuring of
titanium collectors by laser ablation technique: a novel approach to produce micro-patterned scaffolds for tissue engineering appli-cations. Procedia CIRP 65:19–24
3. Ginestra P, Pandini S, Fiorentino A, Benzoni P, Dell’Era P, Ceretti E (2017) Microstructured scaffold for cellular guided orientation: PCL electrospinning on laser ablated titanium collector. CIRP JMST 19:147–157
4. Zhu Z, Garcia-Gancedo L, Flewitt AJ, Xie H, Moussy F, Milne WI (2012) A critical review of glucose biosensors based on carbon nanomaterials: carbon nanotubes and graphene. Sensors 12:5996– 6022
5. Pollack B, Holmberg S, George D, Tran I, Madou M, Ghazinejad M (2017) Nitrogenrich polyacrylonitrile-based graphitic carbons for hydrogen peroxide sensing. Sensors 17:2407
6. Bisht GS, Canton G, Mirsepassi A, Kulinsky L, Oh S, Dunn-Rankin D, Madou M (2011) Controlled continuous pattering of polymeric nanofibers on three-dimensional substrates using low-voltage near-field electrospinning. Nano Lett 11:1831–1837 7. Arshad SN, Naraghi M, Chasiotis I (2011) Strong carbon
nanofi-bers from electrospun polyacrylonitrile. Carbon 49:1710–1719 8. Ra EJ, An KH, Kim KK, Jeong SJ, Lee YH (2015) Anisotropic
electrical conductivity of MWCNT/PAN nanofiber paper. Chem Phys Lett 416:188–193
9. Dumanlı AG, Windle AH (2012) Carbon fibers from cellulosic precursors: a review. J Mater Sci 47:4236–4250
10. Yusof N, Ismail AF (2012) Post spinning and pyrolysis process of polyacrylonitrile (PAN)- based carbon fiber and activated carbon fiber: a review. J Anal App Pyrolysis 93:1–13
11. Singh A, Jayaram J, Madou M, Akbar S (2012) Pyrolysis of nega-t i v e p h o nega-t o r e s i s nega-t s nega-t o f a b r i c a nega-t e c a r b o n s nega-t r u c nega-t u r e s f o r microelectromechanical systems and electrochemical applications. J Electrochem Soc 149:E78–E83
12. Pumera M (2013) Electrochemistry of graphene, graphene oxide and other graphenoids: review. Electrochem Commun 36:14–18 13. Hiremath N, Mays J, Bhat G (2016) Recent developments in carbon
fibers and carbon nanotube-based fibers: a review. Pol Rev 57:339– 368
14. Hiremath N, Evora MC, Naskar AK, Mays J, Bhat G (2017) Polyacrylonitrile nanocomposite fibers from acrylonitrile-grafted carbon nanofibers. Composite Part B: Engineering 130:64–69
15. Prilutsky S, Zussman E, Cohen Y (2018) The effect of embedded carbon nanotubes on the morphological evolution during the car-bonization of poly(acrylonitrile) nanofibers. Nanotechnology 19: 165603
16. Toray Innovation by Chemistry.http://www.torayca.com
17. Mathur RB, Bahl OP, Dhami TL, Chauhan SK (2003) A novel route to realise high degree of graphitization in carbon-carbon com-posites derived from hard carbons. Carbon Science 4(3):111–116 18. Holmberg S, Ghazinejad M, Cho E, George D, Pollack B,
Perebikovsky A, Ragan R, Madou M (2018) Stress-activated py-rolytic carbon nanofibers for electrochemical platforms. Electrochmica Acta 290:639–648
19. Maitra T, Sharma S, Srivastava A, Cho YK, Madou M, Sharma A (2012) Improved graphitization and electrical conductivity of suspended carbon nanofibers derived from carbon nanotube/ poly-acrylonitrile composites by directed electrospinning. Carbon 50: 1753–1761
20. Qiao B, Ding X, Hou X, Wu S (2011) Study on the electrospun CNTs/polyacrylonitrile-based nanofiber composites. J Nanomater.
21. Caia J, Chawlab S, Naraghi M (2016) Microstructural evolution and mechanics of hot-drawn CNT-reinforced polymeric nanofibers. Carbon 109:813–822
22. Shirvanimoghaddam K, Abolhasani MM, Li Q, Khayyam H, Minoo N (2017) Cheetah skin structure: a new approach for carbon-nano-patterning of carbon nanotubes composites part a ap-plied science and manufacturing. https://doi.org/10.1016/j. compositesa.2017.01.023
23. Li X, Qin A, Zhao X, Liu D, Wang H, He C (2015) Drawing dependent structures, mechanical properties and cyclization behav-iors of polyacrylonitrile and polyacrylonitrile/carbon nanotube composite fibers prepared by plasticized spinning. Phys Chem 17: 21856–21865
24. Ginestra PS, Ghazinejad M, Madou M, Ceretti E (2016) Fabrication and characterization of polycaprolactone-graphene powder electrospun nanofibers. Proceeding of SPIE 9932 carbon nanotubes
graphene and emerging 2D materials for electronic and photonic devices IX 99320A
25. Ceretti E, Ginestra PS, Ghazinejad M, Fiorentino A, Madou M (2017) Electrospinning and characterization of polymer-graphene powder scaffolds. CIRP Ann 66(1):233–236
26. Chen R, Liu J, Sun Z, Chen D (2018) Functional Nanofibers with multiscale structure by electrospinning. Nanofabrication 4:17–31 27. Ulubayram K, Calamak S, Shahbazi R, Eroglu I (2015) Nanofibers
based antibacterial drug design, delivery and applications. Curr Pharm Des 21:1930–1943
28. Ginestra PS, Madou M, Ceretti E (2019) Production of carbonized micro-patterns of photolithography and pyrolysis. Precis Eng 55: 137–143
29. Ghazinejad M, Holmberg S, Pilloni O, Oropeza-Ramos L, Madou M (2017) Graphitizing non-graphitizable carbons by stress-induced routes. Sci Rep 7:16551. https://doi.org/10.1038/s41598-017-16424-z
30. Karacan I, Erdogan G (2012) The role of thermal stabilization on the structure and mechanical properties of polyacrylonitrile precur-sor fibers. Fibers Polym 13(7):855–863
31. Malard LM, Pimenta MA, Dresselhaus G, Dresselhaus MS (2009) Raman spectroscopy in graphene. Phys Rep 473:51–87
32. Fitzer E, Müller DJ (1975) The influence of oxygen on the chemical reactions during stabilization of pan as carbon fiber precursor. Carbon 13:63–69
33. Kipling JJ, Sherwood JN, Shooter PV, Thompson NR (1964) Factors influencing the graphitization of polymer carbons. Carbon 1:315–320
34. Cho E, Perebikovsky A, Benice O, Holmberg S, Madou M, Ghazinejad M (2018) Rapid iodine sensing on mechanically treated carbon nanofibers. Sensors 18:1486. https://doi.org/10.3390/ s18051486
Publisher’s note Springer Nature remains neutral with regard to jurisdic-tional claims in published maps and institujurisdic-tional affiliations.